* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project
Download Wang_Natural zealots as effective absorbents
Document related concepts
Chemical Engineering Journal 156 (2010) 11–24 Contents lists available at ScienceDirect Chemical Engineering Journal journal homepage: www.elsevier.com/locate/cej Review Natural zeolites as effective adsorbents in water and wastewater treatment Shaobin Wang a,∗ , Yuelian Peng b a b Department of Chemical Engineering, Curtin University of Technology, GPO Box U1987, Perth, WA 6845, Australia College of Environmental and Energy Engineering, Beijing University of Technology, Beijing 100022, PR China a r t i c l e i n f o Article history: Received 20 May 2009 Received in revised form 8 October 2009 Accepted 9 October 2009 Keywords: Natural zeolite Adsorption Inorganic ions Organics Water treatment a b s t r a c t Natural zeolites are abundant and low cost resources, which are crystalline hydrated aluminosilicates with a framework structure containing pores occupied by water, alkali and alkaline earth cations. Due to their high cation-exchange ability as well as to the molecular sieve properties, natural zeolites have been widely used as adsorbents in separation and puriﬁcation processes in the past decades. In this paper, we review the recent development of natural zeolites as adsorbents in water and wastewater treatment. The properties and modiﬁcation of natural zeolite are discussed. Various natural zeolites around the world have shown varying ion-exchange capacity for cations such as ammonium and heavy metal ions. Some zeolites also show adsorption of anions and organics from aqueous solution. Modiﬁcation of natural zeolites can be done in several methods such as acid treatment, ion exchange, and surfactant functionalisation, making the modiﬁed zeolites achieving higher adsorption capacity for organics and anions. © 2009 Elsevier B.V. All rights reserved. 1. Introduction Nowadays, the world is facing water crisis due to lacking of clean drinking water. With the fast development of various industries, a huge quantity of wastewater has been produced from industrial processes and was discharged into soils and water systems. Wastewater usually contains many pollutants such as cationic and anionic ions, oil and organics, which have poisonous and toxic effects on ecosystems. Removal of these contaminants requires cost effective technologies and a variety of techniques have been developed in the past decades in dealing with wastewater treatment. Currently, adsorption is believed to be a simple and effective technique for water and wastewater treatment and the success of the technique largely depends on the development of an efﬁcient adsorbent. Activated carbon , clay minerals [2,3], biomaterials , zeolites [5,6], and some industrial solid wastes [7,8] have been widely used as adsorbents for adsorption of ions and organics in wastewater treatment. Since the original discovery of zeolitic minerals in a volcanogenic sedimentary rock, zeolitic tuffs have been found in many areas of the world. In the past decades, natural zeolites have found a variety of applications in adsorption, catalysis, building industry, agriculture, soil remediation, and energy [9,10]. It has been estimated that the world natural zeolite consumption is 3.98 Mt and will reach 5.5 Mt in 2010 . ∗ Corresponding author. E-mail address: [email protected] (S. Wang). 1385-8947/$ – see front matter © 2009 Elsevier B.V. All rights reserved. doi:10.1016/j.cej.2009.10.029 Natural zeolites are hydrated aluminosilicate minerals of a porous structure with valuable physicochemical properties, such as cation exchange, molecular sieving, catalysis and sorption. The use of natural zeolites for environmental applications is gaining new research interests mainly due to their properties and signiﬁcant worldwide occurrence. Application of natural zeolites for water and wastewater treatment has been realised and is still a promising technique in environmental cleaning processes. In the past decades, utilisation of natural zeolites has been focussed on ammonium and heavy metal removal due to the nature of ion exchange and some review papers have been appeared [6,12,13]. Apart from the presence of cations in water, anions and organic compounds are widely presented in wastewater. In recent years, natural zeolite and its modiﬁed forms have also been reported for removal of anions and organics from water systems. However, no such a review has been found. In this paper, we will update the recent research in cation adsorption using natural zeolites as well as their modiﬁed forms for removal of anions and organic compounds in water and wastewater treatment. 2. Properties of natural zeolite There are many natural zeolites identiﬁed in the world. Clinoptilolite, mordenite, phillipsite, chabazite, stilbite, analcime and laumontite are very common forms whereas offretite, paulingite, barrerite and mazzite, are much rarer. Among the zeolites, clinoptilolite is the most abundant natural zeolite and is widely used in the world. In zeolite structure, three relatively independent components are found: the aluminosilicate framework, exchangeable 12 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 Table 1 Structural properties of some natural zeolites. Zeolite Chemical formula Structure type Symmetry, space group Clinoptilolite Mordenite Chabazite Phillipsite Scolecite Stilbite Analcime Laumontite Erionite Ferrierite (K2 , Na2 , Ca)3 Al6 Si30 O72 ·21H2 O (Na2 , Ca)4 Al8 Si40 O96 ·28H2 O (Ca, Na2 ,K2 )2 Al4 Si8 O24 ·12H2 O K2 (Ca, Na2 )2 Al8 Si10 O32 ·12H2 O Ca4 Al8 Si12 O40 ·12H2 O Na2 Ca4 Al10 Si26 O72 ·30H2 O Na16 Al16 Si32 O96 ·16H2 O Ca4 Al8 S16 O48 ·16H2 O (Na2 K2 MgCa1.5 )4 Al8 Si28 O72 ·28H2 O (Na2 , K2 , Ca, Mg)3 Al6 Si30 O72 ·20H2 O HEU MOR CHA PHI NAT STI ANA LAU ERI FER Monoclinic, C2/m Orthorhombic, Cmcm Rhombohedral or triclinic P1 Monoclinic, P21 /m Monoclinic,Cc Monoclinic, C2/m Cubic Ia3d Monoclinic, C2/m Hexagonal P63 /mmc Orthorhombic, Immm Monoclinic, P21 /n cations, and zeolitic water. The general chemical formula of zeolites is Mx/n [Alx Siy O2(x+y) ]·pH2 O where M is (Na, K, Li) and/or (Ca, Mg, Ba, Sr), n is cation charge; y/x = 1–6, p/x = 1–4. The primary building block of zeolite framework is the tetrahedron, the centre of which is occupied by a silicon or aluminium atom, with four atoms of oxygen at the vertices. Substitution of Si4+ by Al3+ deﬁnes the negative charge of the framework, which is compensated by monovalent or divalent cations located together with water. The aluminosilicate framework is the most conserved and stable component and deﬁnes the structure type. The water molecules can be present in voids of large cavities and bonded between framework ions and exchangeable ions via aqueous bridges. The water can also serve as bridges between exchangeable cations. Table 1 presents the chemical formula and structure of some important natural zeolites. Zeolites are capable of exchanging ions with external medium, which is the signiﬁcant characteristic of zeolite. Ion exchange proceeds in an isomorphous fashion. The equilibrium ion exchange is expressed by the following equation Z+ zB A A + + zA BLzB ⇔ zA BzB + zB ALzA (1) where zA + and zB + are the valences of the respective cations, and L is deﬁned as a portion of zeolite framework holding unit negative charge. The ion-exchange behaviour of natural zeolite depends on several factors, including the framework structure, ion size and shape, charge density of the anionic framework, ionic charge and con- centration of the external electrolyte solution [9,14]. Due to the formation environment, natural zeolite has varying chemical composition and cation-exchange capacity (CEC). Table 2 shows the chemical composition and cation-exchange capacity of various natural zeolites from the world. It is seen that the CEC is between 0.6 and 2.3 meq/g. 3. Modiﬁcation of natural zeolite The adsorption characteristics of any zeolite are dependent upon the detailed chemical/structural makeup of the adsorbent. The Si/Al ratio, cation type, number and location are particularly inﬂuential in adsorption. These properties can be changed by several chemical treatments to improve separation efﬁciency of raw natural zeolite. Acid/base treatment and surfactant impregnation by ion exchange are commonly employed to change the hydrophilic/hydrophobic properties for adsorption of various ions or organics. 3.1. Acid/base treatment In general, acid washing of natural zeolite may remove impurities that block the pores, progressively eliminate cations to change into H-form and ﬁnally dealuminate the structure. There are two main types of modiﬁcation procedure, which can be used to form proton exchanged zeolite; ammonium exchange followed by calcination and direct ion exchange with dilute acid solution. Ammonium exchange can maintain the stable structure while acid Table 2 Chemical composition and CEC of natural zeoltes in the world. Zeolite Turkey clinoptilolite Iranian clinoptilolite Cuba clinoptilolite Brazil mordenite Italy phillipsite + chabazite Turkey clinoptilolite Chinese clinoptilolite Chilean clinoptilolite + mordenite Turkey clinoptilolite Croatia clinoptilolite Iranian clinoptilolite + mordenite Turkey clinoptilolite Chinese clinoptilolite Turkey clinoptilolite Chinese clinoptilolite Ukrainian clinoptilolite Ukrainian mordenite Slovakian clinoptilolite Croatian clinoptilolite Ukraine clinoptilolite Australian clinoptilolite Chemical composition (%) SiO2 Al2 O3 Fe2 O3 CaO MgO Na2 O K2 O TiO2 70.90 70.00 62.36 67.82 56.42 69.72 65.52 67.00 69.31 64.93 66.5 64.99 68.27 70.00 69.5 67.29 64.56 67.16 55.80 66.7 68.26 12.40 10.46 13.14 14.96 15.8 11.74 9.89 13.00 13.11 13.39 11.81 9.99 7.48 14.00 11.05 12.32 12.02 12.30 13.32 12.3 12.99 1.21 0.46 1.63 0.42 4.08 1.21 1.04 2.00 1.31 2.07 1.3 3.99 1.95 0.75 0.08 1.26 0.95 2.30 1.30 1.05 1.37 2.54 0.2 2.72 1.87 2.42 2.30 3.17 3.20 2.07 2.00 3.11 3.51 2.61 2.50 2.95 3.01 3.58 2.91 5.75 2.10 2.09 0.83 – 1.22 0.18 0.86 0.31 0.61 0.69 1.13 1.08 0.72 1.01 1.87 1.15 0.13 0.29 0.68 1.10 0.70 1.07 0.83 0.28 2.86 3.99 0.32 2.35 0.76 2.31 2.60 0.52 2.40 2.01 0.18 0.68 0.20 2.95 0.66 0.94 0.66 3.90 2.06 0.64 4.46 4.92 1.20 4.47 8.14 4.14 0.88 0.45 2.83 1.30 3.12 1.95 1.69 2.30 1.13 2.76 2.03 2.28 2.35 2.96 4.11 0.089 0.02 – 0.07 0.004 – 0.21 0.20 – – 0.21 – – 0.05 0.14 0.26 0.23 0.17 – – 0.23 CEC (meq/g) Reference 1.6–1.8 – – 2.29 2.12 1.84 1.03 2.05 – 1.45 1.20                      – – – – – 0.64 1.20 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 treatment generally results in dealumination and reduction of thermal stability. Kurama et al.  investigated the conversion of a natural Turkish clinoptilolite to hydrogen form by the two ways, ammonium exchange followed by calcination and direct treatment with HCl. They found that the ion exchange with H+ has a great inﬂuence on the effective pore volume and surface area of clinoptilolite. The pore volume and surface area are increased from 0.13 to 0.25 mL/g and from 35 to 315 m2 /g, respectively. Cakicioglu-Ozkan and Ulku  reported a study of acid treatment of a Bigadic clinoptilolite using HCl solution at varying concentrations (0.032, 0.16, 0.32, 1.6 or 5 M) and temperatures (25, 40, 75 and 100 ◦ C). They found that super-micropore volume was not very sensitive to acid treatment but the Langmuir surface area and ultra-micropore volume depend on the degree of the removal of aluminium from the structure. A natural zeolite, stilbite, from China was treated in hot HCl solution. The modiﬁcation leads to the variation in framework dealumination, resulting in the modiﬁed zeolites with different thermal stabilities and adsorption property. High silica H-STI zeolites prepared with NH4 + exchange and followed by calcination in ﬂuid air exhibit thermal stability up to 1000 ◦ C with open and perfect channel systems. The H-form STI zeolite possesses high ion-exchange capacity of Ag+ . The stability and effective ion-exchange capacity (EfCEC ) of a Mexican clinoptilolite were also investigated upon treatment by acid phosphate solutions. The results show that the pH of the phosphate solutions inﬂuences the stability and EfCEC of the clinoptilolite-rich tuff. At pH 0, the dealumination of the clinoptilolite takes place, it loses crystallinity and its EfCEC diminishes. When the pH is increased to 4 or 6, changes in the crystallinity are not observed and the amount of aluminium is similar to clinoptiloliterich tuff without treatment, but the EfCEC is slightly increased . Three zeolites from Armenia, Georgia and Greece were treated with dilute KOH and subsequently either reacted with HCl or heated at 700 ◦ C. KOH treatment increased slightly speciﬁc surface area and microporosity due to dissolution of amorphous material. Acid treatment increases signiﬁcantly both the speciﬁc surface area and microporosity and decreases the cation-exchange capacity due to partial dissolution of both Si-tetrahedra and free linkages, which yields secondary micropores and destroys speciﬁc exchange sites of the zeolites. Heating decreases both speciﬁc surface area and microporosity . Therefore, it is deduced that acid treatment will reduce the cation-exchange capacity due to dealumination but it can improve capacity and Si/Al ratio offering advantages for the adsorption/separation of non-polar molecules from water or gas ﬂows. 3.2. Surfactant modiﬁcation Due to the net negative charge on the framework, raw natural zeolites usually have little or no afﬁnity for anions and exhibit low adsorption for organics in aqueous solution. To change the surface properties, one modiﬁcation method widely employed is to use organic surfactants. In the past, many investigations have been conducted on modiﬁcation of natural zeolite with cationic surfactants and then use to remove multiple types of contaminants from water. The surfactants are tetramethylammonium [40,41], cetyltrimethylammonium (CTMA)[42,43], hexadecyltrimethylammonium (HDTMA)[40,44–49], octadecyldimethylbenzyl ammonium (ODMBA)[42,50–52], n-cetylpyridinium(CPD) , benzyltetradecyl ammonium (BDTDA) , stearyldimethylbenzylammonium (SDBAC)[54,55], N,N,N,N ,N ,N -hexamethyl-1,9nonanediammonium , and polyhexamethylene-guanidine. It has been found that surfactant modiﬁcation depends on the degree of surfactant adsorption on zeolite. A general model of sorption of ionic surfactants on a solid surface is the formation of 13 Fig. 1. Hemimicelle (A) and admicelle (B) formation by cationic surfactants on zeolite surface . a monolayer or “hemimicelle” at the solid–aqueous interface via strong Coulombic (ionic) bonds at surfactant concentrations at or below its critical micelle concentration (CMC). If the surfactant concentration in solution exceeds the CMC, then the hydrophobic tails of the surfactant molecules associate to form a bilayer or “admicelle” as shown in Fig. 1 . Thus, surfactant-modiﬁed zeolite can have a complex functional groups for positively charged exchange sites formed by the positive groups –NR+ of the surfactant directed towards the surrounding solution in the bilayer. 4. Application for water treatment Surface water, ground water, and industrial or household wastewater contains many different types of pollutants. These pollutants include inorganic and organic compounds and are more or less hazardous to human being, animals and plants. In the following sections, more recent applications of natural zeolites and their modiﬁed forms for removal of various pollutants from water are discussed in detail. 4.1. Ammonium Ammonium is an important nitrogen ion form in aqueous solution. Its pollution mainly comes from municipal sewage, fertiliser factory wastewater and agricultural wastes. Ammonia nitrogen contributes to accelerated eutrophication of lakes and rivers, dissolved oxygen depletion and ﬁsh toxicity in receiving waters. Higher concentration of ammonium will cause a sharp decrease of dissolved oxygen and obvious toxicity on aquatic organisms. In the past decades, various methods of ammoniacal nitrogen removal from waters have been developed; biological treatments and adsorption are the widely used methods. Natural zeolite from 14 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 Table 3 Ammonium adsorption on natural zeolite. Material Capacity (mg/g) Temperature (◦ C) Reference New Zealand clinoptilolite NaOH–clinoptilolite NaHCO3 –clinoptilolite HCl–clinoptilolite New Zealand clinoptilolite New Zealand mordenite Croatian clinoptilolite Croatian clinoptilolite Chinese clinoptilolite Chinese clinoptilolite Chinese Ca–clinoptilolite Chinese clinoptilolite Chinese Na–clinoptilolite Chinese clinoptilolite Bioﬁlm–clinoptilolite Chinese zeolite-microwave Turkish clinoptilolite Turkey clinoptilolite Turkey clinoptilolite Canada clinoptilolite USA clinoptilolite Na–clinoptilolite Ukraine–clinoptilolite Chilean natural zeolite Iranian clinoptilolite 7.1–8.6 7.3–8.4 8.1–9.3 13.4–16.8 8.5 12.2 13.6 7.7–17.6 2.7–3.2 18.5 20.2–26.3 11.2 22.6 12.3–12.9 9.6–13.2 30.6 5.2–8.1 5.7–7.7 14.5–15.4 18.4–22.9 18.5 20.5 6.6–21.5 11.4–14.8 17.8 – – – – – – – – 20 – 20–60 – – 25 25 25 25–55 30 23–70 20 20–21 20–21 – – 28                          various sources was explored as an effective adsorbent. Table 3 summarises NH4 + adsorption capacity on various sourced natural zeolites. Based on the table, it is seen that ammonium adsorption on natural zeolite is 2.7–30.6 mg/g. Cooney et al.  undertook a laboratory study of a natural Australian zeolite, clinoptilolite, to remove ammonium from water. They investigated the equilibria and kinetic characteristics of ammonium exchange in the zeolite under binary and multi-component conditions. The results revealed that the highest ammonium removal efﬁciency was achieved when the zeolite’s exchange sites were converted to the sodium form. For a multi-component system there was a competitive effect between ammonium and other cations such as Ca2+ , Mg2+ , K+ and the zeolite’s selectivity for ammonium ions was over other cations typically present in sewage. Rozic et al.  investigated the removal of ammonium ion from aqueous solutions using a Croatian clinoptilolite and bentonite. The highest removal efﬁciency for N–NH4 + (61.1 wt%) was achieved with the natural zeolite at the lowest initial concentration, i.e. 100 mg N–NH4 + /L. With the increase of the initial concentration of ammoniacal nitrogen, the removal efﬁciency quickly decreased. For the clay, the ammoniacal nitrogen removal efﬁciency was higher in a liquid colloidal state and the acid modiﬁcation of the clay decreased the efﬁciency of ammoniacal nitrogen removal. A clinoptilolite from New Zealand was treated with alkali solutions and evaluated to remove NH4 + ions from a fellmongery wastewater stream . It was found that after treatment the cation-exchange capacity of the natural zeolite was increased by up to 74% and the zeolite could hold a potential maximum of 18.7–20.1 mg NH4 + /g. The presence of other cations in the fellmongery wastewater apparently interfered with NH4 + ion adsorption, resulting in only a small fraction of the CEC getting occupied by the NH4 + ions. The cation-loaded zeolite could be regenerated for NH4 + ion adsorption by leaching with 0.5 M HCl, and NH4 + adsorption remained unaffected after 12 regeneration cycles. Lebedynets et al.  carried out a study of NH4 + sorption from synthetic aqueous solutions by a Ukraine clinoptilolite. NH4 + sorption by the zeolite would be completed within 24 h for all fraction sizes, initial NH4 + ion concentrations and adsorbate volumes. The amounts of NH4 + ions sorbed increased with increasing initial NH4 + concentration and decreasing adsorbate volumes, with the maximum sorption capacity of 11.5 mg/g. Sprynskyy et al.  investigated NH4 + uptake from synthetic aqueous solutions onto raw and pretreated forms of the same clinoptilolite under dynamic conditions. NH4 + uptake onto the zeolite occurred by exchange with Na+ , Ca2+ , and K+ ions. Although Na+ ions were observed to be more easily exchanged for both hydrogen and ammonium ions, the role of Ca2+ ions increased with zeolite saturation by NH4 + ions. The maximum sorption capacity of the clinoptilolite towards NH4 + ions, estimated under dynamic conditions, was signiﬁcantly higher than that measured under static conditions. A recycling study conﬁrmed the importance of external diffusion for ammonium sorption by the clinoptilolite. Preliminary treatment of the sorbent by heat, acid, and NaCl conﬁrmed the predominant importance of the ionexchange mechanism. NaCl treatment of the clinoptilolite showed an improvement of ammonium removal over other treatments. Englert and Rubio  used a Chilean natural zeolite as an adsorbent for ammonia removal from aqueous solutions. The tests showed the particles were negatively charged over a broad pH range with 18.4 mg NH4 + /g cation-exchange capacity. The ammonia removal appeared to proceed through rapid kinetics at neutral pH value, with removal capacities up to 0.68 meq NH4 + /g. Watanabe et al.  carried out a modiﬁcation of Japanese natural zeolites under hydrothermal conditions to improve the effectiveness of the uptake of ammonium ions. The samples were treated with 0.1, 0.3, 1.0 and 3.0 M NaOH solutions at temperatures from 25 to 150 ◦ C under autogenous pressure for 7 days. After the hydrothermal treatment, the transformation of the zeolites to phillipsite, hydroxyl-sodalite and analcime was observed. The treated products, containing mainly phillipsite, took up twice the amount of ammonium ions as the starting materials. The maximum uptake of ammonium ions was 34.6 mg/g. Farkas et al.  studied the adsorption of ammonium ions and organic pollutants on a natural clinoptilolite in the treatment of leakage waters from waste dumps. Without pre-treatment of leakage water, the exchange of NH4 + on the zeolite was found to be 4.2 mg NH4 + /g. After pretreated by activated carbon, the exchange of ammonium ions on the zeolite was increased to 5.7 mg NH4 + /g. In the ammonium solution, the exchange was 17.70 mg NH4 + /g, suggesting that organic pollutants and K+ and Ca2+ ions in leakage water prevented the exchange of NH4 + ions. Jorgensen and Weatherley  investigated three cationic exchangers including natural clinoptilolite, a gel resin (Dowex 50wx8), and a macronet resin (Purolite MN-500) for the removal of ammonia from wastewaters after secondary biological treatment. The results showed that the presence of organic compounds had variable effects on ammonium ion uptake. For the clinoptilolite a very signiﬁcant increase in column breakthrough performance was observed after cycles of exhaustion and regeneration. Regenerated clinoptilolite showed a maximum breakthrough capacity of 450 bed volumes. The kinetic and equilibrium of ammonium ion uptake from aqueous solutions using a Romanian zeolite tuff and synthetic zeolites (5A, 13X and ZSM-5) was reported by Maranon et al. . The inﬂuences of contact time, pH, ammonium concentration, presence of other cations and anion species were investigated. Adsorption capacities of 19 mg NH4 + /g were obtained in multi-component solutions (containing NH4 + , Zn2+ , Cd2+ , Ca2+ , Na+ ). The presence of Zn and Cd at low concentrations did not affect the ammonium adsorption capacity. Comparison between natural and synthetic zeolites, the removal efﬁciencies of ammonium by zeolite tuff were similar to those of zeolites 5A and 13X at low initial ammonium concentration, and much higher than those of zeolite ZSM-5. A study of kinetics and equilibrium isotherms of ammonium ion on a natural Turkish clinoptilolite was also conducted using a batch S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 experimental technique . The effects of relevant parameters, such as temperature, contact time, and initial ammonium concentration were examined. The Langmuir and Freundlich models were applied to describe the equilibrium isotherms for ammonium uptake and the Langmuir model agreed very well with experimental data. Thermodynamic parameters showed that the exchange of ammonium ion by the clinoptilolite is spontaneous and exothermic process. Some natural Chinese clinoptilolites were also tested for ammonia removal. Wang et al.  assessed the application for ammonia removal from the leachate solution of sewage sludge in batch study. The effects of relevant parameters, such as contact time, initial ammonia concentration, and particle size of clinoptilolite, were examined, respectively. The results show that the Langmuir isotherms reﬂect more reasonable for ammonium ion uptake onto the clinoptilolite with the maximum adsorption capacity of 1.74 mg NH4 –N/g. Wen et al.  studied the sorption kinetics of ammonium onto three types of zeolite, natural zeolite, natural zeolite covered by bioﬁlm, and ammonium-bearing zeolite covered by bioﬁlm. Ion exchange between NH4 + and cations in the zeolite increased with decreasing particle size of the zeolite. Bioﬁlm covered on the zeolite did not affect the ion exchange for the smaller particle size but decreased the ion-exchange capacity by 22% for the larger particle size. Bioregeneration could recover 78.0 and 63.9% ion-exchange capacity for the smaller and larger particle size of zeolite, respectively. Equilibrium studies showed that the adsorption system was well ﬁtted by the Freundlich isotherm . Lei et al.  compared the effect of pre-treatment method of a natural Chinese zeolite on ammonium adsorption. Adsorption kinetics, adsorption equilibrium isotherms and the effects of the individual presence of other cations and humic acid on the removal of ammonium were investigated. The zeolite treated under microwave irradiation had the highest ammonium adsorption capacity value, followed by the zeolite obtained by thermal process and the untreated zeolite. Five isotherm models were used to describe the isotherm data and the three-parameter isotherm models (Redlich–Peterson and Langmuir–Freundlich) provided much better ﬁtting to isotherm data than two-parameter isotherm models (Freundlich, Temkin and Langmuir). The presence of Na+ , K+ , Ca2+ and Mg2+ could reduce the uptake of ammonium onto the zeolite treated under microwave irradiation and the order of ammonium ion over other cations was Na+ > K+ > Ca2+ > Mg2+ , while the presence of humic acid increased the uptake of ammonium. A natural Bigadic clinoptilolite was evaluated for NH4 + adsorption . Thermodynamic investigation indicated that ammonium removal by the clinoptilolite was favourable at lower temperatures and exothermic in nature. Different isotherm models were evaluated for ﬁtting the equilibrium data and Khan’s model had better performance for modelling the equilibrium data. Recently, Hedstrom and Amofah  performed column experiments to estimate the ammonium adsorption capacity of clinoptilolite. Results showed the ammonium adsorption capacity increased with decreasing grain size, and the highest experimental adsorption capacity was 2.7 mg NH4 –N/g. The breakthrough occurred immediately due to a too high loading rate. About 23% of adsorbed ammonium could be desorbed by tap water and desorption was more pronounced during saturated conditions. An Iranian natural clinoptilolite for ammonia removal from aqueous solutions has also been thoroughly studied by Ashraﬁzadeh et al. . Both batch and column experiments were carried out. Through the batch experiments, it was found that ammonia removal occurred rapidly within the ﬁrst 15 min of contact time. An adsorption capacity about 17.8 mg NH4 + /g at feed ammonia concentration of 50 mg/L was obtained and the optimum range for pH was about 5.5–7.6. The adsorption capacity of clinoptilolite in the continuous mode was about 15.16 and 15.36 mg NH4 + /g for the original and regenerated 15 types of clinoptilolite, respectively. The presence of cations such as Ca2+ , Mg2+ and Na+ in the feed solution reduced the clinoptilolite adsorption capacity to about 11.68 mg NH4 + /g. It has been shown that the main mechanism that accounts for the adsorption of ammonium ion onto natural zeolites is ion exchange. The results in Table 3 have demonstrated that adsorption capacity of clinoptilolite is 2–30 mg NH4 + /g. Some treatments of clinoptilolite zeolite could increase adsorption capacity, especially after Na+ exchange due to high afﬁnity of NH4 + over Na+ . For other types of natural zeolite, ion exchange with NH4 + is similar to clinoptilolite. The ion-exchange order of zeolite for alkali metal, alkaline earth metal and NH4 + ions is Rb+ > K+ > NH4 + > Ba2+ > Na+ > Ca2+ > Li+ . However, other components in solution such as heavy metal ions and organics will reduce ammonium exchange capacity due to competitive adsorption. Natural zeolite after ammonium adsorption can be regenerated by Na or K ion exchange or by heat treatment for NH3 devolatilisation. 4.2. Heavy metal ions Contamination of heavy metals in water supplies has steadily increased over the last decades as a result of over population and expansion of industrial activities. The presence of heavy metals in the environment is a major concern due to their toxicity. It has been found that many heavy metal ions produce strong health problem and damage to plants and animals. Most of these heavy metals present in polluted waters include Hg, Pb, Ag, Cu, Cd, Cr, Zn, Ni, Co and Mn. In the past, many investigations have been conducted using natural zeolite for metal ion adsorption and several review works have been appeared [12,14]. However, these investigations focussed on single metal ion and the afﬁnity to zeolite. While for real wastewater systems, there are different types of contaminants and may contain a mixture of metal ions. In recent years, more investigations have concentrated in this area. Table 4 presents the adsorption capacity of various metal ions on different natural zeolites. Panayotova  conducted a series of experiments using a Bulgarian natural zeolite and modiﬁed forms for removal of several metal ions such as Ni2+ , Cu2+ , Cd2+ , Zn2+ and Pb2+ . In Ni2+ adsorption, natural and NaOH-, NaCl-, HCl-, and CH3 COONa-modiﬁed zeolites have been tested in a batch process. For raw zeolite, the uptake process obeys the ﬁrst-order irreversible kinetics. The uptake equilibrium is best described by the Langmuir adsorption isotherm. Zeolite modiﬁcation with CH3 COONa and NaCl can increase Ni2+ adsorption by 25–30%. The raw and modiﬁed zeolites will be easily regenerated in 2 M NaCl solution. For Cu2+ removal, uptake of Cu2+ by zeolite from neutral wastewater has proved to be as effective as precipitation of copper hydroxide. The simultaneous presence of Ca2+ and Mg2+ does not signiﬁcantly inﬂuence the uptake of Cu2+ . The uptake equilibrium is best described by the Langmuir adsorption isotherm with maximum adsorption of 6.74 mg/g. The zeolites modiﬁed by NaCl, CH3 COONa and NaOH exhibit higher uptake ability. Kinetics and thermodynamics of uptake of Cd2+ by natural and modiﬁed zeolites have shown the second-order irreversible reactions and the equilibrium data obtained were best ﬁt to Freundlich adsorption isotherm . But uptake of Cd2+ was considerably decreased in the presence of Ca2+ and Mg2+ and the zeolite treated with NaCl and CH3 COONa showed the highest uptake ability. Panayotova and Velikov  further studied the kinetics of the uptake of cadmium, lead, copper, nickel and zinc ions from single ion solutions and from their mixture by the Bulgarian zeolitic rock. It was found that lead ions were strongly immobilised by the zeolite, in single ion and mixed solutions, as well as soft and hard water. Further investigation indicated that pre-treatment of zeolite with NaCl leads to increased rate of heavy metal ions’ immobilisation, as 16 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 Table 4 Adsorption of heavy metal ions on various natural zeolites. Material Metal 2+ Adsorption (meq/g) Reference Sardinian clinoptilolite Cu Cd2+ Pb2+ Zn2+ 0.34 0.05–0.19 0.27–1.2 0.1  Turkish clinoptilolite Pb2+ Zn2+ Cu2+ Ni2+ 0.299–0.730 0.108–0.251 0.022–0.227 0.017–0.173  Natural phillipsite Pb2+ 0.234–0.345  3+ Natural clinoptilolite Cr Ni2+ Zn2+ Cu2+ Cd2+ 0.237 0.068 0.106 0.186 0.082  Clinoptilolite Cd2+ 0.12–0.18  Scolecite Pb2+ Cu2+ Zn2+ Ni2+ , Co2+ Cd2+ 0.056 0.130 0.064 0.031 0.0078 0.0032  Bigadic clinoptilolite Pb2+ Zn2+ Cd2+ 0.222 0.734 0.0053  Mexican clinoptilolite Pb2+ 1.4  Ukraine clinoptilolite Pb2+ Cu2+ Ni2+ Cd2+ 0.134 0.405 0.222 0.0375  Turkish clinoptilolite Co2+ Cu2+ Zn2+ Mn2+ 0.448 0.282 0.268 0.153  Brazilian scolecite Cr3+ Ni2+ Cd2+ Mn2+ 5.81 2.08 1.78 4.00  well as to increased distribution coefﬁcients. However, zeolite pretreatment with NaCl practically does not change zeolite selectivity sequence for the ions in multi-component solutions . Cincotti et al.  examined Sardinian natural clinoptilolites for removal of heavy metals, i.e., lead, cadmium, copper, and zinc in as-received and sodium homoionic forms. A selectivity scale Pb > Cu > Cd ∼ Zn was found based on maximum metal removal. Inglezakis et al.  presented a study of using natural clinoptilolite and bentonite to remove Pb2+ from aqueous solutions. Bentonite was found to be more effective for the removal of Pb2+ than clinoptilolite under the experimental conditions used. The removal of Pb2+ using bentonite reached 100% at ambient temperature and mild agitation (100 rpm) while the highest removal level reached by clinoptilolite was 55%. Clinoptilolite dust is found to be more efﬁcient than granular clinoptilolite. Agitation and temperature affected the uptake of Pb2+ , especially in the case of granular clinoptilolite (2.5–5.0 mm). The adsorption of lead increased with an increase in pH of the solution from 1 to 4. The retention of lead by a Mexican clinoptilolite-rich tuff was evaluated by Llanes-Monter et al. . The maximum Pb2+ exchange capacity of the Mexican clinoptilolite-rich tuff was 1.4 meq/g at pH 3. The chemical lead speciation, the pH, as well as the characteristics of the clinoptilolite-rich tuff are important factors to be considered on the lead sorption process by natural zeolites. Al-Haj-Ali and Al-Hunaidi  studied Pb2+ on a natural phillipsite in a laboratory-scale packed-bed column. Bed depth-service time (BDST) model was applied and parameters for column design were determined for lead ions at 5% breakthrough yielding BDST sorption capacity of 24.3–35.7 mg/g. A natural clinoptilolite from Turkey for the uptake of Pb2+ , Ni2+ , Cu2+ and Zn2+ in single and mixed ion solutions was evaluated by Oter and Akcay . Contact time, initial solution pH, solid-toliquid ratio and initial metal cation concentration were determined as single ion sorption parameters. The maximum adsorption capacity was found as 0.730, 0.251, 0.227 and 0.173 meq/g for Pb2+ , Zn2+ , Cu2+ , Ni2+ , respectively. However, the values from the mixed ion solutions were signiﬁcantly reduced to 0.299, 0.108, 0.022 and 0.017 meq/g for Pb2+ , Zn2+ , Cu2+ , Ni2+ ions, respectively. The clinoptilolite selectivity in both single and mixed ion solution is Pb2+ > Zn2+ > Cu2+ > Ni2+ , which is the similar order to the report of Cincotti et al. . Payne and Abdel-Fattah  conducted batch kinetic and isotherm studies to compare and evaluate different types of adsorbents such as activated carbon and naturally occurring zeolites (clinoptilolite and chabazite) and synthesised zeolites Faujasite (13X) and Linde type A (5A) for Pb2+ removal. The relative rate for lead ion adsorption was: 13X > chabazite > clinoptilolite > 5A > activated carbon. Adsorption isotherm of chabazite and clinoptilolite could be best ﬁt with the Freundlich isotherm. Applications of chabazite and clinoptilolite would require pH values between 4 and 11 and ionic competition reduced lead ion removal by the zeolites. Increasing temperature improved adsorption performance for the zeolites. Sprynskyy et al.  carried out a study on the sorption of heavy metals (Ni2+ , Cu2+ , Pb2+ and Cd2+ ) under static conditions from single- and multi-component aqueous solutions by raw and pretreated clinoptilolites. Fig. 2 presents kinetic adsorption of Ni2+ , Cu2+ , Pb2+ and Cd2+ in single- and multi-component systems. They found the sorption to be an ion-exchange process and consisted of three stages, i.e., the adsorption on the surface of microcrystals, the inversion stage, and the moderate adsorption in the interior of the microcrystal. The ﬁner clinoptilolite fractions adsorbed higher amounts of the metals due to relative enriching by the zeolite proper and higher cleavage. For Cu2+ , Pb2+ and Cd2+ , no difference was observed in single- and multi-component systems. The decrease of nickel adsorption from multi-component solutions was probably caused by the propinquity of its sorption forms to the other metals and by competition. The maximum sorption capacity of Cd2+ is determined as 4.22 mg/g at an initial concentration of 80 mg/L and 27.7, 25.76 and 13.03 mg/g at 800 mg/L for Pb2+ , Cu2+ and Ni2+ . Turkman et al.  studied removal of heavy metals (Pb2+ , Cd2+ , Ni2+ and Zn2+ ) in synthetic and real wastewaters using activated and non-activated natural clinoptilolite. Gordes and Bigadic zeolites in Turkey were used for Cd2+ and Ni2+ removal and their efﬁciencies were compared with that of natural zeolites from other different areas. Although Cd2+ was not removed effectively by Bigadic zeolite, while 46% removal efﬁciency was achieved on Gordes zeolite after 90 min of contact in batch tests. Column studies were also performed for the removal of Pb2+ , Cd2+ and Zn2+ from a lead–zinc mining process raw wastewater. The clinoptilolite exhibited about 100, 98, and 96% removal efﬁciency for Pb2+ , Zn2+ and Cd2+ , respectively. The overall adsorption capacities for Bigadic clinoptilolite were around 23 mg Pb2+ /g, 24 mg Zn2+ /g and 0.6 mg Cd2+ /g. Oren and Kaya  also compared Zn2+ adsorption characteristics of Gordes and Bigadic zeolites. The results showed the removal efﬁciency of Gordes zeolite is two times higher than that of Bigadic zeolite, similar to the above Turkman results. Gedik and Imamoglu  also investigated Cd2+ removal from aqueous solutions using as-received and NaCl-pretreated forms of Gordes and Bigadic zeolites. The maximum sorption capacities for as- S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 17 Fig. 2. Kinetics of metal sorption from single- and multi-component (Cu2+ , Pb2+ , Ni2+ , and Cd2+ ) solutions under static conditions (0.5 g zeolite, fraction 0.71–0.50 mm, 200 mL solution, C0 = 20 mg/L for Cu2+ , Ni2+ , and Pb2+ and C0 = 2 mg/L for Cd2+ , pH 6.2).. received samples were determined as 0.18 and 0.12 meq/g for Gordes and Bigadic zeolites, whereas 0.72 and 0.41 meq Cd/g were determined for their pretreated forms, respectively. Wingenfelder et al.  investigated the removal of Fe, Pb, Cd, and Zn from synthetic mine waters by a natural zeolite. Pb was removed efﬁciently from neutral as well as from acidic solutions, whereas the uptake of Zn and Cd decreased with low pH and high iron concentrations. With increasing Ca concentrations in solution, elimination of Zn and Cd became poorer while removal of Pb remained virtually unchanged. The zeolite was stable in acidic solutions. Disintegration was only observed below pH 2.0. A natural clinoptilolite was modiﬁed to a clinoptilolite–iron oxide system (Clin–Fe) for the removal of Mn2+ , Zn2+  and Cu2+  ions from drinking water samples. Under experimental conditions, the adsorbed maximum amount of Mn for clinoptilolite was 7.69 mg/g whereas that for the Clin–Fe system was 27.1 mg/g. The respective values for the adsorption of Zn were 71.3 and 94.8 mg/g and the maximum adsorbed Cu amount on clinoptilolite was 13.6 mg/g whereas on the Clin–Fe system was 37.5 mg/g. These results indicated an improvement of metal adsorption with iron exchanger. Stefanovic et al.  investigated the effect of pre-treatment of clinoptilolite tuff from Serbia by using NaCl or CaCl2 on Zn2+ adsorption. Pre-treatment of zeolite tuff affects the sorption capac- ity and local structure of Zn2+ . Pre-treatment of clinoptilolite tuff by using NaCl or CaCl2 solutions resulted in a higher zinc uptake comparing to the untreated zeolite sample, i.e. up to 4 wt% of zinc in the clinoptilolite crystals in Na-pretreated form and up to 1.5 or 0.6 wt% of zinc in Ca-pretreated and in untreated zeolite form, respectively. Trgo et al.  investigated the kinetics of zinc and lead ions removal by NaCl-modiﬁed clinoptilolite. The rate of the ion-exchange process for lead ions is faster than for zinc ions. The ion-exchange capacity of zeolite of lead ions is doubly higher than that of zinc ions. Bosso and Enzweiler  evaluated a scolecite for heavy metal removal (Pb2+ , Cu2+ , Zn2+ , Ni2+ , Co2+ and Cd2+ ) from aqueous solutions. The results indicated an afﬁnity order of scolecite for Cu2+ , Zn2+ , Pb2+ , Ni2+ , Co2+ and Cd2+ with a retention value of 130, 64, 56, 31, 7.8 and 3.2 eq/g, respectively. Alvarez-Ayuso et al.  studied the sorption behaviour of natural clinoptilolite and synthetic NaP1 zeolites for Cr3+ , Ni2+ , Zn2+ , Cu2+ and Cd2+ in puriﬁcation of metal ﬁnishing wastewaters. The synthetic zeolite exhibited about 10 times greater sorption capacities than natural zeolite. The adsorption capacity of natural clinoptilolite is 0.079 mmol/g for Cr, 0.034 mmol/g for Ni, 0.053 mmol/g for Zn, 0.093 mmol/g for Cu and 0.041 mmol/g for Cd, respectively. This mineral showed the same high sorption capacity values when used in the puriﬁcation of metal electroplating wastewaters. Table 5 Cation-exchange selectivity of heavy metal ions on natural zeolites. Zeolite Selectivity Si/Al Reference Clinoptilolite Clinoptilolite Clinoptilolite Clinoptilolite Clinoptilolite Phillipsite Mordenite Scolecite Chabazite Pb2+ > Ag+ > Cd2+ ∼ Zn2+ > Cu2+ Pb2+ > Zn2+ > Cu2+ > Ni2+ Pb2+ > Cd2+ > Zn2+ ∼ Cu2 Pb2+ > Cd2+ > Cu2+ > Co2+ > Cr3+ > Zn2+ > Ni2+ > Hg2+ Pb2+ > Fe3+ > Cu2+ > Zn2+ ∼ Cd2+ ∼ Co2+ > Ni2+ > Mn2+ > Cr3+ Pb2+ > Cd2+ > Zn2+ > Co2+ Mn2+ > Cu2+ > Co2+ ∼ Zn2+ > Ni2+ Cu2+ > Zn2+ > Pb2+ > Ni2+ > Co2+ > Cd2+ Pb2+ > Cd2+ > Cu2+ > Zn2+ > Co2+ 2.7–5.3 4.9 4.2 – – 2.4–2.7 4.4–5.5 1.56 2.2–2.6          18 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 Table 6 Kinetic parameters for adsorption of heavy metal ions on natural zeolites. Zeolite Metal ion 2+ Reaction order First-order rate constant (min−1 ) Second-order rate constant (g/mg h) Reference Clinoptilolite Cd Pb2+ Ni2+ Cu2+ Zn2+ Firs-order 0.0137 0.0532 0.0158 0.0200 0.0210  Clinoptilolite Chabazite Pb2+ Pb2+ First-order First-order 2.9 × 10−4 4.3 × 10−4   Clinoptilolite Pb2+ Ni2+ First-order 0.0053 0.1419  Clinoptilolite Pb2+ First-order 3.5 × 10−4 Scolecite Mn2+ Cr3+ Ni2+ Cd2+ Second-order 0.0155 0.0365 0.0248 0.0503  Clinoptilolite Cu2+ Cd2+ Second-order 0.00113 0.0226  Akgul et al.  have recently investigated the removal of silver ions from aqueous solution using a natural clinoptilolite. They carried out batch experiments to examine the effects of various parameters such as pH, adsorption time, metal ion concentration and the acidic treatment on the adsorption process. They found that acid treatment has a substantial effect on the metal uptake. Adsorption phenomena appeared to follow the Langmuir and Freundlich isotherms and Ag+ maximum adsorption capacity was 33.23 mg Ag+ /g. For ion exchange with various heavy metals in wastewater systems, cation selectivity of zeolite is important for selective ion removal. Table 5 shows cation-exchange selectivity of important heavy metal ions on several natural zeolites. As seen that Pb has the higher afﬁnity for ion exchange for most of zeolites. Other metal ions show varying order depending on the type of zeolite. It is noted that ion-exchange selectivity also depends on the ion concentration and solution pH. Therefore, these factors should be taken into consideration in real wastewater treatment. For zeolite application in heavy metal adsorption, ion-exchange kinetics is also important. Previous investigations have showed that adsorption of heavy metal ions generally follow two kinetic models, pseudo-ﬁrst-order or pseudo-second-order. Table 6 gives some results of previous investigations. It is seen that the kinetics of heavy metal depends on zeolite type and metal ions. 4.3. Inorganic anions Inorganic anions contain several acid ions and some metalloid and metal anions. The acid ions such as NO3 − , SO4 2− , PO4 3− , F− , ClO4 − , CN− are largely present in wastewater. These ions can cause pollution at high content. Other important inorganic anions include Cr(V) with CrO4 2− , Cr2 O7 2− forms, and As(V) with H2 AsO4 2− , HAsO4 − , and As(III), which are strong toxic species in water system. Currently, removal of anions using natural zeolites can be achieved on ion-exchanged zeolite and surfactant-modiﬁed forms. For acid anions, natural zeolite has been tested for F− and CN− adsorption. Diaz-Nava et al.  evaluated the sorption of ﬂuoride ions on a natural Mexican heulandite–clinoptilolite. In their work, the effects of sodium, calcium, lanthanum, and europium in the crystalline network as well as the effects of pH and particle size of the zeolite on the ﬂuoride sorption were investigated. They found that retention of ﬂuoride was similar for the untreated material and treated samples with sodium, calcium, lanthanum, and europium. The ﬂuoride retention was proposed as occlusion and adsorption  of ﬂuoride on zeolite. Samatya et al.  also prepared metal ion (Al3+ , La3+ and ZrO2+ ) exchanged zeolites for ﬂuoride removal from water on a Turkish clinoptilolite. The natural zeolite samples were pre-conditioned with HNO3 (ZEO-1), NaNO3 (ZEO-2), and deionised water (ZEO-3) before loading Al3+ , La3+ and ZrO2+ . They found that ZEO-1 type zeolite had a higher capacity than ZEO-2 and ZEO-3 type zeolites. Equilibrium isotherms ﬁtted well to the Langmuir and Freundlich models. Percent removal of ﬂuoride from aqueous solution containing 2.5 mg F/L was 94% using metal loaded zeolite (ZEO-1) at an adsorbent concentration of 6.00 g/L. For Al3+ , La3+ and ZrO2+ exchanged zeolites, ﬂuoride adsorption capacity follows the order of Zr-Zeo > La-Zeo > Al-Zeo. Faghihian  described the preparation and evaluation of various modiﬁed metal forms of clinoptilolite for removal of cyanide from aqueous solutions. The cobalt form of the zeolite showed the highest uptake of 1.95 meq/g-zeolite whereas the uptake on natural forms is 0.070 meq/g. It has been known that metal chromium is a highly toxic metal. Its presence in water is generally in Cr3+ and Cr(VI). Compared with Cr3+ , Cr(VI) state is of particular concern due to its higher toxicity. Since earlier work of Haggerty and Bowman  using surfactant to modify surface charge of zeolite for anion adsorption, a lot of investigations have been carried out. Ghiaci et al.  compared the performance of synthetic and natural zeolites modiﬁed by surfactant HDTMA and CPB as well as MCM-41 molecular sieve for removal of chromate from aqueous solution. HDTMA- and CPC-clinoptilolite exhibit higher adsorption than ZSM-5 based adsorbents, but less than MCM-41. The maximum chromate adsorption on HDTMA- and CPC-clinoptilolite is dependent on surfactant loading in a range of 4.4–16.6 and 3.9–21.4 mmol/kg, respectively. Campos et al.  investigated the modiﬁed-natural mordenite using HDTMA and ethylhexadecyldimethylammonium (EHDDMA) as adsorbents for the removal of Cr (VI) from aqueous solution. The results showed that the HDTMA-HSO4 modiﬁed zeolite exhibited higher adsorption for Cr(VI) than EHDDMA-modiﬁed zeolite. The sorption of chromate on HDTMA-zeolite resulted from a combination of entropic, coulombic, hydrophobic effects, and HDTMA counterion. Cordoves et al.  also reported a study of a surfactant-modiﬁed clinoptilolite (SMZ) in the removal of Cr(VI) and Cr3+ . The cation and anion exchange capacities of each zeolite were obtained. It has been demonstrated that the afﬁnity distribution analysis combined with the Freundlich binding model allows the characterization of the SMZ binding properties for Cr(VI). In comparison to other surfactant-modiﬁed clinoptilolites, this activated zeolite proved S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 to have improved properties for Cr(VI) adsorption, providing a method for separation of Cr(VI) from Cr3+ . Wingenfelder et al.  employed HDTMA-modiﬁed zeolite for sorption of antimonate. During the modiﬁcation, the zeolite sorbed more than 94% of HDTMA. Desorption of HDTMA from the zeolite was less than 15% in total after threefold washing with distilled water. Antimonate binding was most effective on the zeolite treated with HDTMA solutions exceeding the zeolites external cation-exchange capacity. Antimonate sorption on modiﬁed zeolite was best described by the Langmuir isotherms. HDTMA-zeolite in aqueous suspension (50 g/L) sorbed up to 42% of antimonate from solutions containing from 0.09 to 2.15 mmol Sb/L. Elizalde-Gonzalez et al.  investigated arsenic sorption on clinoptilolites from Mexico and Hungary. Both clinoptilolites are able to decrease the initial arsenic concentration of 200 g/L by more than 75% in deionised, drinking, ground and surface waters. In the case of the Mexican zeolite, both the arsenite and the arsenate concentrations (200 g/L) can be lowered from 200 to 10 g/L. It was found that the presence of cations and anions in the natural waters did not reduce the efﬁciency of the selected zeolites. The Hungarian zeolite removed 75% of the arsenate and only 50% when the sample was ﬁrst acidiﬁed. This zeolite totally desorbed the ﬁxed arsenic into a water volume. Dousova et al.  studied the sorption of arsenate from aqueous solution on three adsorbents, metakaoline, clinoptilolite-rich tuff, and synthetic zeolite, in both untreated and Fe2+ -treated forms. It was found that the sorption capacity of Fe2+ -treated sorbents increased signiﬁcantly from about 0.5 to >20.0 mg/g, which represented more than 95% of the total As removal. Habuda-Stanic et al.  compared different modiﬁed adsorbents (zeolite–clinoptilolite, manganese greensand and cationic exchange resin) for arsenic removal from contaminated drinking water. Adsorbents were chemically modiﬁed and saturated with Fe3+ ions, while the arsenic solutions were prepared by processed groundwater. Adsorption tests show that Fe3+ saturated zeolite is effective for arsenic removal with capacity of 55.3 g/g for As(III) and 36.4 g/g for As(V). Macedo-Miranda and Olguin  reported arsenic sorption onto Mexico clinoptilolite-heulandite rich tuffs modiﬁed with lanthanum, hexadecyltrimethylammonium or iron. The Langmuir isotherm presented the arsenic (V) sorption capacity of the zeolites as 75.4 g As/g at pH 3, 3.9 g As/g at pH 5 and 53.6 g As/g at pH 6, for the lanthanum, HDTMA and iron modiﬁed clinoptiloliteheulandite rich tuff, respectively. In general, the results suggested that the arsenic retention depends on the precedence of zeolitic material, the nature of arsenic chemical species, pH as well as the characteristics of modiﬁed-natural zeolites. Davila-Jimenez et al.  introduced iron species into a clinoptilolite-rich zeolitic tuff using different organic and inorganic iron salts after pre-treatment with NaCl. The introduced iron corresponded to four coordinated species with tetrahedral geometry, primarily low spin ferric iron adsorbing almost 12 g/g arsenite (99% removal) from a 360 g(As(III))/L and 6 g/g arsenate from a 230 g(As(V))/L. Adsorption of arsenite and arsenate reached practically a plateau at Fe/Si = 0.1 in the series of exchanged tuffs. The oxidation of arsenite to arsenate in the solution in contact with iron modiﬁed tuff during adsorption was observed by speciation. 4.4. Organics Organic contaminants are important pollutants in water. The removal of dyes and organics in an economic way remains an important problem although a number of systems have been developed with adsorption techniques. Adsorption has been found to be superior to other techniques for water re-use in terms of ini- 19 Table 7 Dye adsorption on natural zeolite. Material Dye Adsorption (mg/g) Reference Clinoptilolite Clinoptilolite Clinoptilolite HTAB-clinoptilolite HTAB-clinoptilolite HTAB-clinoptilolite CTAB-clinoptilolite CTAB-clinoptilolite Clinoptilolite HTAB-clinoptilolite CTAB-clinoptilolite Clinoptilolite Methylene blue Rhodamine B Malachite green Reactive black 5 Reactive red 239 Reactive yellow 176 Reactive black 5 Reactive red 239 Basic red 46 Reactive yellow 176 Reactive yellow 176 Toluidine blue O 19.9 12.4 19.7 60.6 111.1 88.5 12.1–12.9 11.0–15.9 8.6 13.2 5.5 33.0–58.7             tial cost, simplicity of design, ease of operation and insensitivity to toxic substances. 4.4.1. Dye adsorption Dyes are important pollutants in wastewater, which are mainly discharged from textile, printing, food and leather industries. Various types of dyes including basic, acidic, reactive, and dispersive dyes are widely used. Dyes in waters affect the nature of the water, inhibiting sunlight penetration into the stream and reducing the photosynthetic reaction. Some dyes are also toxic and even carcinogenic . In the past years, some investigations using natural zeolites for dye adsorption have been reported and Table 7 presents the adsorption capacities of various dyes on natural zeolites. Meshko et al.  investigated the adsorption of two basic dyes, MG-300 and MG-400 with components of (2-[[(4-methoxyphenyl)methylhydrazono]methyl]-1,3,3-trimethylindolium methosulfat and 2-[[4-[ethyl(2-hydroxyethyl) amino]phenyl]azo]-6methoxy-3-methylbenzothiazoliumchloride), onto granular activated carbon and natural clinoptiolite. The inﬂuences of agitation, initial dye concentration and adsorbent mass were studied using batch reactor. The equilibrium studies showed that both dyes have higher adsorption capacity for the granular activated carbon than for the natural zeolite. Homogeneous diffusion model combined with external mass transfer resistance was proposed for the kinetic investigation. The adsorption capacities of two dyes on natural zeolite are 55.9 and 14.9 mg/g, respectively. Armagan et al. [111–115] conducted a comprehensive study on a Turkey clinoptillolite for adsorption of three reactive azo dyes (reactive black 5, reactive red 239, and reactive yellow 176) and compared the adsorption with a clay sample, sepiolite. The adsorption results indicated that both natural sepiolite and zeolite have limited adsorption capacities of the reactive dyes. After modiﬁcation with quaternary amines (hexadecyltrimethylammonium bromide. HTAB), the adsorption was signiﬁcantly improved. An electrostatic adsorption mechanism involving the formation of a bilayer of amine molecules on the clinoptilolite surface onto which anionic dye molecules adsorb was proposed. The adsorption data were ﬁtted to the Langmuir isotherm and the modiﬁed zeolite produced adsorption capacities of 111, 89, and 61 mg/g for reactive red, yellow and black, respectively. Benkli et al.  also investigated HTAB-modiﬁed clinoptilolite for removal of reactive azo dyes, reactive black 5, red 239 and yellow 176, in a ﬁxed bed. The results indicated the order of dye removal by modiﬁed zeolite in the following manner: black > yellow > red. Calculations of the HTAB coverage on zeolite surface indicate that a bilayer formation is the most viable packing that enables maximum removal of the dyes. Karadag et al.  also studied raw zeolite and surfactantmodiﬁed zeolite for adsorption of basic red 46 (BR46) and reactive yellow 176 (RY176) and compared the effect of different surfactants of cetyltrimethylammonium bromide (CTAB) and hex- 20 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 adecyltrimethylammonium bromide (HTAB) on dye adsorption. BR46 adsorption onto natural zeolite increased to minor extent with increasing pH, whereas pH did not signiﬁcantly affect RY176 adsorption. The increase in ionic strength caused a decrease in adsorption of BR46 and an increase in adsorption of RY176. Adsorption of BR46 on natural zeolite is more favourable than RY176 on the CTAB and HTAB modiﬁed zeolites. They  further investigated CTAB modiﬁed-natural zeolite for other reactive dye adsorption. The adsorption capacity of Reactive Red 239 was found to be two times higher than Reactive Blue 5 due to the hydrophilicity of the dye molecules. The pseudo-second-order model provided a very good ﬁtting for the two anionic dyes. The calculated maximum adsorption capacity increased with increasing initial dye concentration, but there is no linear relationship with pH and temperature. Alpat et al.  also used the Turkish clinoptilolite for the adsorption of toluidine blue O (TBO). Kinetic studies showed that adsorption of TBO on the clinoptilolite was ﬁtted to the second-order adsorption model with two-step diffusion process. The activation energies for TBO adsorption on clinoptilolite for the ﬁrst and second diffusion processes were 8.72 and 19.02 kJ/mol, respectively. The adsorption isotherm was well ﬁtted to both the Langmuir and Freundlich models. The maximum adsorption capacity of clinoptilolite for TBO was 2.1 × 10−4 mol/g at solution pH of 11.0. An Australian natural clinoptiloite was tested for basic dye adsorption . The natural zeolite presented maximal adsorption capacity of 2.8 × 10−5 and 7.9 × 10−5 mol/g at 50 ◦ C for Rhodamine B and methylene blue, respectively. Kinetic studies indicated that the adsorption followed the pseudo-second-order kinetics and could be described as two-stage diffusion process. It has also found that the regenerated zeolites by high-temperature calcination and Fenton oxidation showed similar adsorption capacity but lower than the fresh sample. Only 60% capacity could be recovered by the two regeneration techniques . Wang and Ariyanto  also investigated the competitive adsorption of malachite green and Pb2+ ions from aqueous solution on the Australian natural zeolite. For single system, malachite green adsorption isotherm follows the Langmuir model and the adsorption capacity is 5 × 10−5 mol/g. In the binary system, malachite green and Pb2+ exhibit competitive adsorption on the natural zeolite. The adsorption is reduced to 90 and 80% of single component of Pb2+ and malachite green, respectively. However, the total adsorption is higher. In the binary system, Pb2+ exhibits relative higher afﬁnity and selectivity to be adsorbed on zeolite. The dynamic adsorption of malachite green and Pb2+ still follows the ﬁrst-order kinetics. Han et al.  studied methylene blue adsorption on a Chinese natural zeolite in column tests under different ﬂow rates and initial concentrations and estimated the kinetic parameters. The results showed that natural zeolite was efﬁcient to remove methylene blue from solution. The breakthrough data were ﬁtted to Thomas model equations. From the above investigations, it is found that natural zeolites are effective for cationic dye adsorption due to the cation-exchange characteristic while they exhibits low capacity in anionic dyes. After surfactant modiﬁcation, natural zeolites will be good adsorbents for anionic dye adsorption. 4.4.2. Humic substances Humic substances make up about 80% of soil organic matters in dark soils. Most humic substances are resulted from the natural process of plant matter decay. Humic substances have been designated as either humic acid, fulvic acid or humin. The presence of humic substance in surface and ground water will produce toxic chemicals during disinfection processes and thus should be removed. Many techniques have been developed for removal of humic substance. Some investigators have also employed natu- Table 8 HA adsorption on natural zeolites. Adsorbent Capacity (mg/g) Temperature (◦ C) pH Reference NYT Na-NYT K-NYT NH4-NYT Ca-NYT Mg-NYT Ba-NYT CLT Ca-CLT NYT Ca-NYT Australian 8.51 6.70 6.58 7.02 21.5 22.0 11.3 2.35 2.60 17.1 22.5 68 30 30 30 30 30 30 30 RT RT RT RT 30 – – – – – – – 7.2 7.2 7.2 7.2 5.0             ral zeolite for removal of humic substance by adsorption. Table 8 presents a summary of previous investigation results. Wang et al.  reported an investigation of modiﬁcation of clinoptilolite surface (SMZ) with HDTMA to improve the removal efﬁciency of fulvic acids (FA). They investigated the effects of relevant parameters such as HDTMA loading levels, FA ﬂow rate and efﬂuent concentration in a ﬁxed bed. FA adsorption on SMZ surfaces is largely due to the hydrophobic interaction and hydrogen bonding. Optimisation studies showed that the SMZ bed with HDTMA loading of 120% of ECEC at a ﬂow rate of 5 BV/h had the best performance and the volume of 23 BV of 30 vol% ethanol solution with the feed ﬂow rate of 5 BV/h was sufﬁcient for complete regeneration of the SMZ. Capasso et al.  studied the interaction of humic acid (HA) with zeolitic (phillipsite + chabazite) Neapolitan yellow tuff (NYT). HA sorption isotherms were carried out on untreated as well as on Li+ -, Na+ -, K+ -, NH4 + -, Ca2+ - or Ba2+ -enriched samples. They obtained maximum HA sorbable amount and the afﬁnity constant between sorbate and the sorbent. Fig. 3 shows the adsorption isotherms of humic acid on various zeolites. The results demonstrated that enrichment by divalent cations enhances the ability of NYT to take up humic acid, whereas enrichment by monovalent cations reduces the adsorption. The results also showed that humic acid sorption on tuff must be regarded as a complex phenomenon, occurring as a compromise between the ability of the cations to form stable bridges with the organic matter and, on the other hand, their speciﬁc selective sorption by the ruff. They  further tested the ability of NYT enriched with calcium ions to remove humic acids from water by batch and column experiments. The sorption capacity increased with the ionic strength and has the highest value at pH 7.4. They  also compared the sorption of humic acids (HA) on Caenriched NYT and a clinoptilolite-rich tuff from Turkey (CLT). NYT sorption capacity was higher than that of CLT. HA sorption by Caenriched NYT readily attained a pseudo steady-state, after which the tuff/HA-solution system evolved in a few months to a ﬁnal equilibrium state characterized by a much higher sorption capability. Desorption experiments at high pH levels resulted in a HA recovery >80%. Wang et al.  studied the adsorption of humic acid (HA) on an Australian natural zeolite tuff. The adsorption capacity of humic acid at 30 ◦ C with pH 5 was found as 68 mg/g. Solution pH inﬂuenced humic acid adsorption. In Pb2+ /HA system, Pb2+ exhibits competitive adsorption with humic acid on the natural zeolite, resulting in reduced adsorption of both Pb2+ and humic acid. However, in Cu2+ /HA system, competitive adsorption and complexation between Cu2+ and humic acid inﬂuence the adsorption, resulting in decreased adsorption of humic acid but increased adsorption of Cu2+ . The complexation structure of Pb–HA/zeolite and Cu–HA/zeolite in three-component system was proposed as S–Pb–HA and S–HA–Cu, respectively. S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 21 Fig. 4. BTEX breakthrough curves for HDTMA-modiﬁed zeolite column saturation, oilﬁeld water experiment . Fig. 3. Humic acid adsorption on untreated zeolite tuff and on various cationenriched tuff samples . Therefore, it is seen that natural zeolite can also be used as an adsorbent for humic substance adsorption. However, the adsorption capacity depends on the structure and chemical composition of natural zeolite. 4.4.3. Other organics Apart from dyes and natural organic matter, wastewater usually contains other organic compounds, such as phenolic compounds, petroleum, surfactants, pesticides, and pharmaceuticals, which are from various industrial sources. These organics are generally more toxic than dyes and humic substance and removal of these organic compounds is more important in water and wastewater treatment. However, removal of organics from water using natural zeolite is usually involved of surfactant modiﬁcation of zeolite. Li and Bowman  investigated the sorption of a non-polar organics, perchloroethylene (PCE), on HDTMA-modiﬁed zeolite (SMZ). Below monolayer coverage by the surfactant, the PCE sorption coefﬁcient on SMZ was proportional to the fractional organic carbon content. Above monolayer coverage, increasing fractional organic carbon content resulted in minimal further increase in the PCE sorption coefﬁcient. They also determined the sorption of ionisable organic solutes, benzene, phenol and aniline on SMZ . The sorption was affected by solution pH. Phenol sorption by SMZ treated to bilayer coverage increased with the pH and hence fraction of anionic phenolate increased. The counterion balance indicated that the increased retention of phenol was due partially to anion exchange of phenolate for bromide, the same mechanism responsible for sorption of inorganic anions by SMZ. In contrast, decreases in pH resulted in reduced aniline sorption due to a lower concentration of the neutral species and repulsion of the positively charged anilinium from SMZ treated to bilayer coverage. Huttenloch et al.  investigated chlorosilanes modiﬁednatural diatomite and zeolite materials for sorption of toluene, o-xylene, and naphthalene from water. Trimethylchlorosilane (TMSCI), tert-butyldimethylchlorosilane (TBDMSCI), dimethyloctadecylchlorosilane (DMODSCI), and diphenyldichlorosilane (DPDSCI) were used. Sorption tests showed enhanced adsorption on the surface modiﬁcation materials compared to the untreated ones which showed no measurable sorption. Batch sorption experiments showed that the phenyl head groups of DPDSCI have the best afﬁnity for aromatic compounds. Removal from an aqueous solution of 10 mg/L of naphthalene, o-xylene, and toluene was 51, 30, and 16% for modiﬁed clinoptilolite, respectively. Ersoy and Celik  investigated the adsorption of aniline and nitrobenzene on natural zeolite and HDTMA-modiﬁed zeolite (OZ). In batch tests, the adsorption capacity of aniline and nitrobenzene onto natural zeolite surface is very low or almost nil but becomes signiﬁcant on OZ. In the column tests, adsorption capacity of two compounds on OZ from the breakthrough curves was determined as 2.36 and 3.25 mg/g for aniline and nitrobenzene, respectively. Ghiaci et al.  prepared organo-zeolites, ZSM-5 and natural zeolites with HDTMA and n-cetylpyridinium bromide (CPB), and tested for adsorption of nonionic organic contaminants (NOCs) such as benzene, toluene, and phenol from contaminated wastewater. They found that the increase in NOCs concentration or initial concentrations of surfactants resulted in an increase in the NOC adsorption. At a certain concentration, CPB modiﬁed zeolite showed higher adsorption than that of the corresponding HDTMA-modiﬁed zeolite. Organo-natural clinoptilolite exhibits higher sorption capacity of NOCs than organo-ZSM-5. A study for evaluation of HDTMA-modiﬁed zeolite (SMZ) for removal of BTEX from produced water was reported by Ranck et al. . The results showed that SMZ completely removes BTEX and that SMZ can be regenerated via air sparging without loss of sorption capacity. The ﬁeld-scale system was also tested at a natural gas produced-water treatment facility. In the ﬁeld column, initial benzene breakthrough occurred at 10 PV and toluene breakthrough began at 15 PV and no breakthrough of ethylbenzene or xylenes occurred throughout the 80 PV experiment. Bowman  evaluated a HDTMA-modiﬁed zeolite in a permeable reactive barrier for the removal of contaminants from sub-surface water. A 15-week pilot test showed barrier retardation factors of 44 and 39 for chromate and PCE, respectively, similar to the values predicted from laboratory experiments. He also tested the HDTMA-modiﬁed zeolite for removal of organics present in oilﬁeld wastewaters. Fig. 4 shows the ﬁrst BTEX saturation experiment. As expected, the higher solubility species benzene and toluene appear ﬁrst in the efﬂuent and reach inﬂuent concentrations relatively rapidly, followed by the more hydrophobic, 22 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24 more strongly retained ethylbenzene and xylenes which take much longer to reach inﬂuent concentrations. The total mass of BTEX retained by the SMZ-ﬁlled column is 65.3 mg for benzene, 148 mg for toluene, 628 mg for methylbenzene, 698 mg for m-, p-xylene, and 657 mg for o-xylene, respectively. Laboratory and ﬁeld experiments also showed that SMZ removed 99–100% of bacteria and viruses present in sewage efﬂuent. Systematic adsorption tests were carried out to determine the efﬁciency of SDBAC-modiﬁed zeolite for removal of pesticides, atrazine, lindane and diazinone from water . The effects of adsorbent particle size, solid content in the suspension and the initial pesticide concentration in the solutions were investigated. The adsorption capacities, calculated by ﬁtting the experimental data to the Langmuir–Freundlich equation, were 2.0 mol/g (atrazine), 4.4 mol/g (diazinone) and 3.4 mol/g (lindan). Column experiments showed that at volumetric ﬂow of 6 cm3 /min, the breakthrough points (at C/C0 = 0.1) were 560 bed volume (BV) for lindane and 620 for diazinone. Dakovic et al.  investigated the adsorption of ochratoxin A (OCHRA) on clinoptilolite-heulandite rich tuff modiﬁed with ODMBA at different amounts 20, 50 and 100 mol/g, which were denoted as OZ-2, OZ-5 and OZ-10. They found that adsorption of OCHRA on organo-zeolites is dependent on the amount of organic cation at the surface as well as on their surface concentrationarrangement of alkyl chains at the surface. High surface coverage of ODMBA resulted in higher OCHRA adsorption. At low surface concentration of ODMBA, OCHRA adsorption was pH dependent while at higher concentrations of ODMBA adsorption of both neutral and anionic forms of OCHRA occurred. They also investigated the adsorption of zearalenone (ZEN)  and fumonisin B-1 (FB1)  on OZ-2, OZ-5, and OZ-10. Results showed that the presence of ODMBA ions at the zeolite surface greatly improved adsorption of ZEN and FB1. The pH signiﬁcantly inﬂuenced ZEN and FB1 adsorption. The estimated maximum FB1 adsorption to OZ-10, based on a Langmuir model, was 10.82 mg/g at pH 3. Kuleyin  investigated the adsorption of phenol and 4chlorophenol on HDTMA- and BDTDA-modiﬁed zeolite. Phenol and 4-chlorophenol removal efﬁciency by the surfactant-modiﬁed zeolite was higher than natural zeolite. The phenol removal efﬁciencies reached up to 71 and 73% for HDTMA-zeolite and BDTDA-zeolite and the 4-chlorophenol removal efﬁciencies reached up to 81 and 89% for HDTMA-zeolite and BDTDA-zeolite at 50 mg/L. Therefore, natural zeolite exhibits little adsorption of organics in aqueous solution due to its surface hydrophilics. Surfactant modiﬁcation can change the surface functionality by adding hydrophobic groups and thus enhancing adsorption capacity of various organics. However, the adsorption depends on surfactant loading and coverage on zeolite. 5. Conclusion and future perspectives Natural zeolites are important low cost materials for water and wastewater treatment. Due to the nature of cation exchange, natural zeolites exhibit high performance in adsorption of cations in aqueous solution such as ammonium and heavy metals. However, zeolites show varying ion selectivity and competitive adsorption for a multi-component system. In addition, these materials are not good adsorbents for adsorption of anionic ions and organics. Surface modiﬁcation using cationic surfactant can change the surface charge of natural zeolite, making them applicable for adsorption of anions and organics. Modiﬁcation of natural zeolites using some heavy metals can also make them for inorganic anion adsorption by surface precipitation. Natural zeolite for cationic ion adsorption has been intensively investigated; however, its modiﬁed forms using surfactants for anionic ion adsorption have not been comprehensively car- ried out. Detailed mechanism of contaminant/surfactant/zeolite interactions is required for better design of surfactant-modiﬁed zeolite. In addition, regeneration of spent zeolite using simple methods for adsorbent recycling should also be a focus in future research. In the past, most tests using natural zeolites were based on batch mode, focussing on their applicability and selectivity. However, once batch conditions, adsorptive capacity and the uptake mechanism are established work should be directed to design and carry out some pilot-plant scale studies to check their feasibility at industrial level. More important, real wastewater should be tested instead of synthetic wastewater. References  S.J.T. Pollard, G.D. Fowler, C.J. Sollars, R. Perry, Low-cost adsorbents for waste and waste-water treatment—a review, Science of the Total Environment 116 (1992) 31–52.  M.R.M.P. de Aguiar, A.C. Novaes, A.W.S. Guarino, Removal of heavy metals from wastewaters by aluminosilicate, Quimica Nova 25 (2002) 1145–1154.  G. Crini, Non-conventional low-cost adsorbents for dye removal: a review, Bioresource Technology 97 (2006) 1061–1085.  G. Crini, Recent developments in polysaccharide-based materials used as adsorbents in wastewater treatment, Progress in Polymer Science 30 (2005) 38–70.  S. Babel, T.A. Kurniawan, Low-cost adsorbents for heavy metals uptake from contaminated water: a review, Journal of Hazardous Materials 97 (2003) 219–243.  A. Hedstrom, Ion exchange of ammonium in zeolites: a literature review, Journal of Environmental Engineering: ASCE 127 (2001) 673–681.  S.B. Wang, H.W. Wu, Environmental-benign utilisation of ﬂy ash as low-cost adsorbents, Journal of Hazardous Materials 136 (2006) 482–501.  S. Wang, H.M. Ang, M.O. Tadé, Novel applications of red mud as coagulant, adsorbent and catalyst for environmentally benign processes, Chemosphere 72 (2008) 1621–1635.  D.L. Bish, D.W. Ming, Applications of natural zeolites in water and wastewater treatment, Natural Zeolites: Occurrence, Properties, Applications 45 (2001) 519–550.  G.V. Tsitsishvili, T.G. Andronikashvili, G.N. Kirov, L.D. Filizova, Natural Zeolites, E. Horwood, New York, 1992.  S. Ozaydin, G. Kocar, A. Hepbasli, Natural zeolites in energy applications, Energy Sources Part A: Recovery Utilization and Environmental Effects 28 (2006) 1425–1431.  S. Kesraouiouki, C.R. Cheeseman, R. Perry, Natural zeolite utilization in pollution-control—a review of applications to metals efﬂuents, Journal of Chemical Technology and Biotechnology 59 (1994) 121–126.  D. Caputo, F. Pepe, Experiments and data processing of ion exchange equilibria involving Italian natural zeolites: a review, Microporous and Mesoporous Materials 105 (2007) 222–231.  D. Kallo, Applications of natural zeolites in water and wastewater treatment, in: D.L. Bish, D.W. Ming (Eds.), Natural Zeolites: Occurrence, Properties, Applications (2001) 519–550.  S.K. Alpat, O. Ozbayrak, S. Alpat, H. Akcay, The adsorption kinetics and removal of cationic dye, Toluidine Blue O, from aqueous solution with Turkish zeolite, Journal of Hazardous Materials 151 (2008) 213–220.  S.N. Ashraﬁzadeh, Z. Khorasani, M. Gorjiara, Ammonia removal from aqueous solutions by Iranian natural zeolite, Separation Science and Technology 43 (2008) 960–978.  C. Cabrera, C. Gabaldon, P. Marzal, Sorption characteristics of heavy metal ions by a natural zeolite, Journal of Chemical Technology and Biotechnology 80 (2005) 477–481.  V. Campos, L.C. Morais, P.M. Buchler, Removal of chromate from aqueous solution using treated natural zeolite, Environmental Geology 52 (2007) 1521–1525.  S. Capasso, S. Salvestrini, E. Coppola, A. Buondonno, C. Colella, Sorption of humic acid on zeolitic tuff: a preliminary investigation, Applied Clay Science 28 (2005) 159–165.  S. Capasso, E. Coppola, P. Iovino, S. Salvestrini, C. Colella, Sorption of humic acids on zeolitic tuffs, Microporous and Mesoporous Materials 105 (2007) 324–328.  Q. Du, S. Liu, Z. Cao, Y. Wang, Ammonia removal from aqueous solution using natural Chinese clinoptilolite, Separation and Puriﬁcation Technology 44 (2005) 229–234.  A.H. Englert, J. Rubio, Characterization and environmental application of a Chilean natural zeolite, International Journal of Mineral Processing 75 (2005) 21–29.  E. Erdem, N. Karapinar, R. Donat, The removal of heavy metal cations by natural zeolites, Journal of Colloid and Interface Science 280 (2004) 309–314.  A. Farkas, M. Rozic, Z. Barbaric-Mikocevic, Ammonium exchange in leakage waters of waste dumps using natural zeolite from the Krapina region, Croatia, Journal of Hazardous Materials 117 (2005) 25–33. S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24  M. Ghiaci, R. Kia, A. Abbaspur, F. Seyedeyn-Azad, Adsorption of chromate by surfactant-modiﬁed zeolites and MCM-41 molecular sieve, Separation and Puriﬁcation Technology 40 (2004) 285–295.  A. Gunay, Application of nonlinear regression analysis for ammonium exchange by natural (Bigadic) clinoptilolite, Journal of Hazardous Materials 148 (2007) 708–713.  Z.-Y. Ji, J.-S. Yuan, X.-G. Li, Removal of ammonium from wastewater using calcium form clinoptilolite, Journal of Hazardous Materials 141 (2007) 483– 488.  D. Karadag, Y. Koc, M. Turan, M. Ozturk, A comparative study of linear and nonlinear regression analysis for ammonium exchange by clinoptilolite zeolite, Journal of Hazardous Materials 144 (2007) 432–437.  L.C. Lei, X.J. Li, X.W. Zhang, Ammonium removal from aqueous solutions using microwave-treated natural Chinese zeolite, Separation and Puriﬁcation Technology 58 (2008) 359–366.  O. Korkuna, R. Leboda, J. Skubiszewska-Zieba, T. Vrublevs’ka, V.M. Gun’ko, J. Ryczkovski, Structural and physicochemical properties of natural zeolites: clinoptilolite and mordenite, Microporous and Mesoporous Materials 87 (2006) 243–254.  K. Pilchowski, E. Chmielewská, Adsorptive separation of 1,2-dichloroethane from model wastewater by natural clinoptilolite, Acta Hydrochimica et Hydrobiologica 31 (2003) 249–252.  M. Rozic, S. Cerjan-Stefanovic, S. Kurajica, V. Vancina, E. Hodzic, Ammoniacal nitrogen removal from water by treatment with clays and zeolites, Water Research 34 (2000) 3675–3681.  M. Sprynskyy, M. Lebedynets, A.P. Terzyk, P. Kowalczyk, J. Namiesnik, B. Buszewski, Ammonium sorption from aqueous solutions by the natural zeolite Transcarpathian clinoptilolite studied under dynamic conditions, Journal of Colloid and Interface Science 284 (2005) 408–415.  S.B. Wang, Z.H. Zhu, Characterisation and environmental application of an Australian natural zeolite for basic dye removal from aqueous solution, Journal of Hazardous Materials 136 (2006) 946–952.  H. Kurama, A. Zimmer, T. Reschetilowski, Chemical modiﬁcation effect on the sorption capacities of natural clinoptilolite, Chemical Engineering & Technology 25 (2002) 301–305.  F. Cakicioglu-Ozkan, S. Ulku, The effect of HCl treatment on water vapor adsorption characteristics of clinoptilolite rich natural zeolite, Microporous and Mesoporous Materials 77 (2005) 47–53.  X.W. Cheng, Y. Zhong, J. Wang, J. Guo, Q. Huang, Y.C. Long, Studies on modiﬁcation and structural ultra-stabilization of natural STI zeolite, Microporous and Mesoporous Materials 83 (2005) 233–243.  N.A. Hernandez-Beltran, M.T. Olguin, A. Rosas-Aburto, Effect of acid phosphate media on the stability of clinoptilolite-rich tuff, Journal of Inclusion Phenomena and Macrocyclic Chemistry 61 (2008) 93–100.  G.E. Christidis, D. Moraetis, E. Keheyan, L. Akhalbedashvili, N. Kekelidze, R. Gevorkyan, H. Yeritsyan, H. Sargsyan, Chemical and thermal modiﬁcation of natural HEU-type zeolitic materials from Armenia, Georgia and Greece, Applied Clay Science 24 (2003) 79–91.  S.C. Bouffard, S.J.B. Duff, Uptake of dehydroabietic acid using organicallytailored zeolites, Water Research 34 (2000) 2469–2476.  E.J. Sullivan, J.W. Carey, R.S. Bowman, Thermodynamics of cationic surfactant sorption onto natural clinoptilolite, Journal of Colloid and Interface Science 206 (1998) 369–380.  D. Karadag, E. Akgul, S. Tok, F. Erturk, M.A. Kaya, M. Turan, Basic and reactive dye removal using natural and modiﬁed zeolites, Journal of Chemical and Engineering Data 52 (2007) 2436–2441.  D. Karadag, M. Turan, E. Akgul, S. Tok, A. Faki, Adsorption equilibrium and kinetics of reactive black 5 and reactive red 239 in aqueous solution onto surfactant-modiﬁed zeolite, Journal of Chemical and Engineering Data 52 (2007) 1615–1620.  Y.E. Benkli, M.F. Can, M. Turan, M.S. Celik, Modiﬁcation of organo-zeolite surface for the removal of reactive azo dyes in ﬁxed-bed reactors, Water Research 39 (2005) 487–493.  R.S. Bowman, Applications of surfactant-modiﬁed zeolites to environmental remediation, Microporous and Mesoporous Materials 61 (2003) 43– 56.  R. Cortes-Martinez, V. Martinez-Miranda, M. Solache-Rios, I. Garcia-Sosa, Evaluation of natural and surfactant-modiﬁed zeolites in the removal of cadmium from aqueous solutions, Separation Science and Technology 39 (2004) 2711–2730.  R. Cortes-Martinez, M. Solache-Rios, V. Martinez-Miranda, R. Alfaro-Cuevas, Sorption behavior of 4-chlorophenol from aqueous solutions by a surfactantmodiﬁed Mexican zeolitic rock in batch and ﬁxed bed systems, Water Air and Soil Pollution 183 (2007) 85–94.  G.M. Haggerty, R.S. Bowman, Sorption of chromate and other inorganic anions by organo-zeolite, Environmental Science & Technology 28 (1994) 452–458.  A. Kuleyin, Removal of phenol and 4-chlorophenol by surfactant-modiﬁed natural zeolite, Journal of Hazardous Materials 144 (2007) 307–315.  A. Dakovic, M. Tomasevic-Canovic, G. Rottinghaus, V. Dondur, Z. Masic, Adsorption of ochratoxin A on octadecyldimethyl benzyl ammonium exchanged-clinoptilolite-heulandite tuff, Colloids and Surfaces B: Biointerfaces 30 (2003) 157–165.  A. Dakovic, M. Tomasevic-Canovic, G.E. Rottinghaus, S. Matijasevic, Z. Sekulic, Fumonisin B-1 adsorption to octadecyldimethylbenzyl ammonium-modiﬁed clinoptilolite-rich zeolitic tuff, Microporous and Mesoporous Materials 105 (2007) 285–290. 23  A. Dakovic, S. Matijasevic, G.E. Rottinghaus, V. Dondur, T. Pietrass, C.F.M. Clewett, Adsorption of zearalenone by organomodiﬁed natural zeolitic tuff, Journal of Colloid and Interface Science 311 (2007) 8–13.  M. Ghiaci, A. Abbaspur, R. Kia, F. Seyedeyn-Azad, Equilibrium isotherm studies for the sorption of benzene, toluene, and phenol onto organo-zeolites and as-synthesized MCM-41, Separation and Puriﬁcation Technology 40 (2004) 217–229.  J. Lemic, M. Tomasevic-Canovic, M. Adamovic, D. Kovacevic, S. Milicevic, Competitive adsorption of polycyclic aromatic hydrocarbons on organo-zeolites, Microporous and Mesoporous Materials 105 (2007) 317–323.  J. Lemic, D. Kovacevic, M. Tomasevic-Canovic, D. Kovacevic, T. Stanic, R. Pfend, Removal of atrazine, lindane and diazinone from water by organo-zeolites, Water Research 40 (2006) 1079–1085.  M. Noroozifar, M. Khorasani-Motlagh, M.N. Gorgij, H.R. Naderpour, Adsorption behavior of Cr(VI) on modiﬁed natural zeolite by a new bolaform N,N,N,N ,N ,N -hexamethyl-1,9-nonanediammonium dibromide reagent, Journal of Hazardous Materials 155 (2008) 566–571.  P. Misaelides, D. Zamboulis, P. Sarridis, J. Warchol, A. Godelitsas, Chromium (VI) uptake by polyhexamethylene-guanidine-modiﬁed natural zeolitic materials, Microporous and Mesoporous Materials 108 (2008) 162– 167.  E.L. Cooney, N.A. Booker, D.C. Shallcross, G.W. Stevens, Ammonia removal from wastewaters using natural Australian zeolite. I. Characterization of the zeolite, Separation Science and Technology 34 (1999) 2307–2327.  N.S. Bolan, C. Mowatt, D.C. Adriano, J.D. Blennerhassett, Removal of ammonium ions from fellmongery efﬂuent by zeolite, Communications in Soil Science and Plant Analysis 34 (2003) 1861–1872.  M. Lebedynets, M. Sprynskyy, I. Sakhnyuk, R. Zbytniewski, R. Golembiewski, B. Buszewski, Adsorption of ammonium ions onto a natural zeolite: Transcarpathian clinoptilolite, Adsorption Science & Technology 22 (2004) 731–741.  Y. Watanabe, H. Yamada, J. Tanaka, Y. Moriyoshi, Hydrothermal modiﬁcation of natural zeolites to improve uptake of ammonium ions, Journal of Chemical Technology and Biotechnology 80 (2005) 376–380.  T.C. Jorgensen, L.R. Weatherley, Continuous removal of ammonium ion by ion exchange in the presence of organic compounds in packed columns, Journal of Chemical Technology and Biotechnology 81 (2006) 1151–1158.  E. Maranon, M. Ulmanu, Y. Fernandez, I. Anger, L. Castrillon, Removal of ammonium from aqueous solutions with volcanic tuff, Journal of Hazardous Materials 137 (2006) 1402–1409.  D. Karadag, Y. Koc, M. Turan, B. Armagan, Removal of ammonium ion from aqueous solution using natural Turkish clinoptilolite, Journal of Hazardous Materials 136 (2006) 604–609.  Y.Q. Wang, S.J. Liu, Z. Xu, T.W. Han, S. Chuan, T. Zhu, Ammonia removal from leachate solution using natural Chinese clinoptilolite, Journal of Hazardous Materials 136 (2006) 735–740.  D.H. Wen, Y.S. Ho, X.Y. Tang, Comparative sorption kinetic studies of ammonium onto zeolite, Journal of Hazardous Materials 133 (2006) 252–256.  D.H. Wen, Y.S. Ho, S.G. Xie, X.Y. Tang, Mechanism of the adsorption of ammonium ions from aqueous solution by a chinese natural zeolite, Separation Science and Technology 41 (2006) 3485–3498.  L.R. Weatherley, N.D. Miladinovic, Comparison of the ion exchange uptake of ammonium ion onto New Zealand clinoptilolite and mordenite, Water Research 38 (2004) 4305–4312.  Y.F. Wang, F. Lin, W.Q. Pang, Ammonium exchange in aqueous solution using Chinese natural clinoptilolite and modiﬁed zeolite, Journal of Hazardous Materials 142 (2007) 160–164.  C.H. Liu, K.V. Lo, Ammonia removal from composting leachate using zeolite. I. Characterization of the zeolite, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 36 (2001) 1671–1688.  X.J. Guo, L. Zeng, X.M. Li, H.S. Park, Removal of ammonium from RO permeate of anaerobically digested wastewater by natural zeolite, Separation Science and Technology 42 (2007) 3169–3185.  A. Hedstrom, L.R. Amofah, Adsorption and desorption of ammonium by clinoptilolite adsorbent in municipal wastewater treatment systems, Journal of Environmental Engineering and Science 7 (2008) 53–61.  M. Panayotova, Kinetics and thermodynamics of removal of nickel ions from wastewater by use of natural and modiﬁed zeolite, Fresenius Environmental Bulletin 10 (2001) 267–272.  M.I. Panayotova, Kinetics and thermodynamics of copper ions removal from wastewater by use of zeolite, Waste Management 21 (2001) 671–676.  M. Panayotova, Use of zeolite for cadmium removal from wastewater, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 35 (2000) 1591–1601.  M. Panayotova, B. Velikov, Kinetics of heavy metal ions removal by use of natural zeolite, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 37 (2002) 139–147.  M. Panayotova, B. Velikov, Inﬂuence of zeolite transformation in a homoionic form on the removal of some heavy metal ions from wastewater, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 38 (2003) 545–554.  A. Cincotti, A. Mameli, A.M. Locci, R. Orru, G. Cao, Heavy metals uptake by Sardinian natural zeolites: Experiment and modeling, Industrial & Engineering Chemistry Research 45 (2006) 1074–1084. 24 S. Wang, Y. Peng / Chemical Engineering Journal 156 (2010) 11–24  V.J. Inglezakis, M.A. Stylianou, D. Gkantzou, M.D. Loizidou, Removal of Pb(II) from aqueous solutions by using clinoptilolite and bentonite as adsorbents, Desalination 210 (2007) 248–256.  M.M. Llanes-Monter, M.T. Olguin, M.J. Solache-Rios, Lead sorption by a Mexican, clinoptilolite-rich tuff, Environmental Science and Pollution Research 14 (2007) 397–403.  A. Al-Haj-Ali, T. Al-Hunaidi, Breakthrough curves and column design parameters for sorption of lead ions by natural zeolite, Environmental Technology 25 (2004) 1009–1019.  O. Oter, H. Akcay, Use of natural clinoptilolite to improve, water quality: sorption and selectivity studies of lead(II), copper(II), zinc(II), and nickel(II), Water Environment Research 79 (2007) 329–335.  K.B. Payne, T.M. Abdel-Fattah, Adsorption of divalent lead ions by zeolites and activated carbon: effects of pH, temperature, and ionic strength, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 39 (2004) 2275–2291.  M. Sprynskyy, B. Buszewski, A.P. Terzyk, J. Namiesnik, Study of the selection mechanism of heavy metal (Pb2+ , Cu2+ , Ni2+ , and Cd2+ ) adsorption on clinoptilolite, Journal of Colloid and Interface Science 304 (2006) 21–28.  A.E. Turkman, S. Aslan, I. Ege, Treatment of metal containing wastewaters by natural zeolites, Fresenius Environmental Bulletin 13 (2004) 574–580.  A.H. Oren, A. Kaya, Factors affecting adsorption characteristics of Zn2+ on two natural zeolites, Journal of Hazardous Materials 131 (2006) 59–65.  K. Gedik, I. Imamoglu, Afﬁnity of clinoptilolite-based zeolites towards removal of Cd from aqueous solutions, Separation Science and Technology 43 (2008) 1191–1207.  U. Wingenfelder, C. Hansen, G. Furrer, R. Schulin, Removal of heavy metals from mine waters by natural zeolites, Environmental Science & Technology 39 (2005) 4606–4613.  M.K. Doula, Removal of Mn2+ ions from drinking water by using clinoptilolite and a clinoptilolite–Fe oxide system, Water Research 40 (2006) 3167–3176.  A. Dimirkou, Uptake of Zn2+ ions by a fully iron-exchanged clinoptilolite. Case study of heavily contaminated drinking water samples, Water Research 41 (2007) 2763–2773.  A. Dimirkou, M.K. Doula, Use of clinoptilolite and an Fe-overexchanged clinoptilolite in Zn2+ and Mn2+ removal from drinking water, Desalination 224 (2008) 280–292.  S.C. Stefanovic, N.Z. Logar, K. Margeta, N.N. Tusar, I. Arcon, K. Maver, J. Kovac, V. Kaucic, Structural investigation of Zn2+ sorption on clinoptilolite tuff from the Vranjska Banja deposit in Serbia, Microporous and Mesoporous Materials 105 (2007) 251–259.  M. Trgo, J. Peric, N.V. Medvidovic, A comparative study of ion exchange kinetics in zinc/lead-modiﬁed zeolite–clinoptilolite systems, Journal of Hazardous Materials 136 (2006) 938–945.  S.T. Bosso, J. Enzweiler, Evaluation of heavy metal removal from aqueous solution onto scolecite, Water Research 36 (2002) 4795–4800.  E. Alvarez-Ayuso, A. Garcia-Sanchez, X. Querol, Puriﬁcation of metal electroplating waste waters using zeolites, Water Research 37 (2003) 4855–4862.  M. Akgul, A. Karabakan, O. Acar, Y. Yurum, Removal of silver (I) from aqueous solutions with clinoptilolite, Microporous and Mesoporous Materials 94 (2006) 99–104.  S.M. Dal Bosco, R.S. Jimenez, W.A. Carvalho, Removal of toxic metals from wastewater by Brazilian natural scolecite, Journal of Colloid and Interface Science 281 (2005) 424–431.  S. Wang, E. Ariyanto, Competitive adsorption of malachite green and Pb ions on natural zeolite, Journal of Colloid and Interface Science 314 (2007) 25–31.  C. Diaz-Nava, M.T. Olguin, M. Solache-Rios, Water deﬂuoridation by Mexican heulandite–clinoptilolite, Separation Science and Technology 37 (2002) 3109–3128.  S. Samatya, U. Yuksel, M. Yuksel, N. Kabay, Removal of ﬂuoride from water by metal ions (Al3+ , La3+ and ZrO2+ ) loaded natural zeolite, Separation Science and Technology 42 (2007) 2033–2047.  H. Faghihian, Removal of cyanide from liquid wastes by modiﬁed clinoptilolite, International Journal of Environment and Pollution 22 (2004) 732–739.  A.I.P. Cordoves, M.G. Valdes, J.C.T. Fernandez, G.P. Luis, J.A. Garcia-Calzon, M.E.D. Garcia, Characterization of the binding site afﬁnity distribution of a surfactant-modiﬁed clinoptilolite, Microporous and Mesoporous Materials 109 (2008) 38–48.  U. Wingenfelder, G. Furrer, R. Schulin, Sorption of antimonate by HDTMAmodiﬁed zeolite, Microporous and Mesoporous Materials 95 (2006) 265–271.  M.P. Elizalde-Gonzalez, J. Mattusch, R. Wennrich, Application of natural zeolites for preconcentration of arsenic species in water samples, Journal of Environmental Monitoring 3 (2001) 22–26.  B. Dousova, T. Grygar, A. Martaus, L. Fuitova, D. Kolousek, V. Machovic, Sorption of As (V) on alumino silicates treated with Fe-II nanoparticles, Journal of Colloid and Interface Science 302 (2006) 424–431.  M. Habuda-Stanic, M. Kules, B. Kalajdzic, Z. Romic, Quality of groundwater in eastern Croatia. The problem of arsenic pollution, Desalination 210 (2007) 157–162.  M.G. Macedo-Miranda, M.T. Olguin, Arsenic sorption by modiﬁed clinoptilolite-heulandite rich tuffs, Journal of Inclusion Phenomena and Macrocyclic Chemistry 59 (2007) 131–142.  M.M. Davila-Jimenez, M.P. Elizalde-Gonzalez, J. Mattusch, P. Morgenstern, M.A. Perez-Cruz, Y. Reyes-Ortega, R. Wennrich, H. Yee-Madeira, In situ and ex situ study of the enhanced modiﬁcation with iron of clinoptilolite-rich zeolitic tuff for arsenic sorption from aqueous solutions, Journal of Colloid and Interface Science 322 (2008) 527–536.  S.B. Wang, Y. Boyjoo, A. Choueib, Z.H. Zhu, Removal of dyes from aqueous solution using ﬂy ash and red mud, Water Research 39 (2005) 129–138.  V. Meshko, L. Markovska, M. Mincheva, A.E. Rodrigues, Adsorption of basic dyes on granular acivated carbon and natural zeolite, Water Research 35 (2001) 3357–3366.  B. Armagan, Factors affecting the performances of sepiolite and zeolite for the treatment of textile wastewater, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 38 (2003) 883–896.  B. Armagan, O. Ozdemir, M. Turan, M.S. Celik, The removal of reactive azo dyes by natural and modiﬁed zeolites, Journal of Chemical Technology and Biotechnology 78 (2003) 725–732.  B. Armagan, M. Turan, M.S. Celik, Equilibrium studies on the adsorption of reactive azo dyes into zeolite, Desalination 170 (2004) 33–39.  B. Armagan, M. Turan, O. Ozdemir, M.S. Celik, Color removal of reactive dyes from water by clinoptilolite, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 39 (2004) 1251–1261.  B. Armajan, Factors affecting the performances of sepiolite and zeolite for the treatment of textile wastewater, Journal of Environmental Science and Health Part A: Toxic/Hazardous Substances & Environmental Engineering 38 (2003) 883–896.  S.B. Wang, H.T. Li, S.J. Xie, S.L. Liu, L.Y. Xu, Physical and chemical regeneration of zeolitic adsorbents for dye removal in wastewater treatment, Chemosphere 65 (2006) 82–87.  R.P. Han, Y. Wang, W.H. Zou, Y.F. Wang, H. Shi, Comparison of linear and nonlinear analysis in estimating the Thomas model parameters for methylene blue adsorption onto natural zeolite in ﬁxed-bed column, Journal of Hazardous Materials 145 (2007) 331–335.  S.G. Wang, W.X. Gong, X.W. Liu, B.Y. Gao, Q.Y. Yue, Removal of fulvic acids using the surfactant modiﬁed zeolite in a ﬁxed-bed reactor, Separation and Puriﬁcation Technology 51 (2006) 367–373.  S. Capasso, C. Colella, E. Coppola, P. Iovino, S. Salvestrini, Removal of humic substances from water by means of calcium-ion-enriched natural zeolites, Water Environment Research 79 (2007) 305–309.  S. Wang, T. Terdkiatburana, M.O. Tadé, Adsorption of Cu(II), Pb(II) and humic acid on natural zeolite tuff in single and binary systems, Separation and Puriﬁcation Technology 62 (2008) 64–70.  Z.H. Li, R.S. Bowman, Sorption of perchloroethylene by surfactant-modiﬁed zeolite as controlled by surfactant loading, Environmental Science & Technology 32 (1998) 2278–2282.  Z.H. Li, T. Burt, R.S. Bowman, Sorption of ionizable organic solutes by surfactant modiﬁed zeolite, Environmental Science & Technology 34 (2000) 3756–3760.  P. Huttenloch, K.E. Roehl, K. Czurda, Sorption of nonpolar aromatic contaminants by chlorosilane surface modiﬁed natural minerals, Environmental Science & Technology 35 (2001) 4260–4264.  B. Ersoy, M.S. Celik, Uptake of aniline and nitrobenzene from aqueous solution by organo-zeolite, Environmental Technology 25 (2004) 341–348.  J.M. Ranck, R.S. Bowman, J.L. Weeber, L.E. Katz, E.J. Sullivan, BTEX removal from produced water using surfactant-modiﬁed zeolite, Journal of Environmental Engineering: ASCE 131 (2005) 434–442.